- Email: [email protected]

Contents lists available at ScienceDirect

Opto-Electronics Review journal homepage: http://www.journals.elsevier.com/opto-electronics review

Full Length Article

Ternary photonic crystal with left-handed material layer for refractometric application S.A. Taya Physics Department, Islamic University of Gaza, Palestine

a r t i c l e

i n f o

Article history: Received 31 August 2017 Received in revised form 9 May 2018 Accepted 22 May 2018 Keywords: Photonic crystal Left-handed material Sensor Refractometry application

a b s t r a c t A ternary photonic crystal with left-handed material (LHM) layer is examined for refractometric applications. One of the layers is assumed to be air and treated as an analyte. The transmittance from the ternary photonic crystal is studied in details and the wavelength shift due to the change in the refractive index of the analyte is investigated. The transmittance is investigated with the parameters of the LHM. It is found that the wavelength shift can be signiﬁcantly enhanced with the decrease of both real part of the LHM permittivity and thickness. © 2018 Association of Polish Electrical Engineers (SEP). Published by Elsevier B.V. All rights reserved.

1. Introduction Many researchers were attracted to photonic crystals in recent years due to possible applications in optoelectronics [1–4]. This multilayer structure led to the construction of photonic band gaps which are sometimes called stop bands. The propagation of waves with deﬁnite frequency in these bands is not allowed. The width of this band depends on the incidence angle of light, the indices of refraction of the layers and their thicknesses. If all these parameters are maintained constant, then this one-dimensional photonic crystal structure will possess ﬁxed predetermined forbidden bands of deﬁnite frequencies. Electromagnetic waves of frequency lying in these bands will be reﬂected by the structure. Photonic crystals can be grouped into categories depending on the number of media in one cell. They can be sorted into binary, ternary, quaternary or so on. This classiﬁcation is mainly dependent on the number of media in one period. The binary photonic crystal comprises two media in the period, the ternary has three media in a period, the quaternary has four media in a period and so on. These periods are repeated many times to form photonic band gap structures. Ternary photonic crystal structures have received much more interest because of their excellent performance over the binary photonic crystal structures as sensors for refractometric applications [5], omni-directional reﬂectors [6–8] and optical ﬁlters [9]. The ternary photonic structures may be constructed by the rep-

etition of three materials. The one-dimensional binary photonic crystal can be created by the repetition of two media. The onedimensional ternary photonic band gap structures exhibit also superior temperature sensing elements [10]. Materials are described by their permittivity ε and permeability . Some materials have simultaneous negative electric permittivity and magnetic permeability . Those materials have received high interest due to the possibility of being used in many ﬁelds. They were referred to as left-handed materials (LHMs) because the electric ﬁeld E, magnetic ﬁeld H and wave vector K constitute a left-handed set. LHMs were ﬁrst studied theoretically by the Russian physicist Veselago in 1968 [11]. They have many properties which are different from normal materials with positive ε and . Pendry et al. was the ﬁrst to show the possibility of LHM design by some novel man-made materials [12,13]. Shelby et al. fabricated the ﬁrst LHM in 2001 [14]. Since his wonderful discovery, slab waveguide structures having left-handed material layer have become an interesting topic [15]. Using a slab waveguide as optical sensors is the most recent application of waveguides. They have been utilized as efﬁcient sensors for environmental monitoring, pharmaceutical industry, and food technology. They have many advantages over other sensors such as immunity to light interference [16], fast response, reduced weight and size, resistance to aggressive environments, and easy to interface with optical data communication systems. One of the advantages of slab waveguides and optical ﬁbers is their immunity to electromagnetic interference. It is well known that all metal cable network media have a common problem since they are at risk of electromagnetic interference. Slab waveguides

E-mail address: [email protected] https://doi.org/10.1016/j.opelre.2018.05.002 1230-3402/© 2018 Association of Polish Electrical Engineers (SEP). Published by Elsevier B.V. All rights reserved.

S.A. Taya / Opto-Electronics Review 26 (2018) 236–241

237

connected to the incidence angle 0 through

cos1 =

2

1−

n20 sin 0

Fig. 1. Ternary photonic crystal with three layers having the indices n1 , n2 and n3 .

and optical ﬁbers do not suffer from that problem because they are immune to crosstalk since they do not conduct electricity and guide light signals in a dielectric medium rather than electrical signals along a metallic conductor, to transmit data. So they cannot produce a magnetic ﬁeld result in immune to electromagnetic interference. In 1989, Tiefenthaler et al. studied a slab waveguide for humidity sensing by measuring the change in the effective index of refraction due to any variation in the material contained in the cladding [17]. Since then, considerable research has been conducted to miniature the system and enhance the sensitivity of slab waveguide sensors. Moreover, optical ﬁbers have been used in biosensing in the past few years [18,19]. Surface plasmon resonance (SPR) has been proposed in the ﬁeld of refractometry [20–22]. Metal-clad waveguide (MCWG) design is one of the most commonly used structures as an optical sensor [23–25]. MCWG structure is the same as a waveguide structure of three layers with an extra metal layer. The metal layer is usually sandwiched between the semi-inﬁnite substrate and the core ﬁlm. Waveguide sensors are recognized as evanescent ﬁeld sensors because the evanescent wave is responsible for the sensing operation [26,27]. Any change in the analyte index causes a change in the modal index of the guided mode. In this work, we report the use of one-dimensional ternary photonic crystal in optical sensing applications. The layers of the ternary photonic crystal are dielectric / LHM / air repeated N times in a periodic structure. The transmission spectrum from the proposed structure is investigated and the wavelength shift due to the change in the refractive index of air is calculated with different parameters of the structure. To the best of my knowledge, this is the ﬁrst time an LHM is used as a layer in a ternary photonic crystal for optical sensing applications and this is the novel scientiﬁc contribution of the current work.

⎡ l cosˇi ⎣ M [d] =

−isinˇi pi

−ipi sinˇi

Where l = 3, 1 =

n20 sin 0 (n3 )2

2

n20 sin 0

12

n22

12 .

The derivation of matrix M is provided in Appendix A. of Inspection the determinant of the matrix M[d] in Eq. (1), we ﬁnd that M[d] = 1. If the system under consideration has N periods, the characteristic matrix is written as

N

[M (d)] =

where

M12 TN−1 (a)

M21 TN−1 (a)

M22 TN−1 (a) − TN−2 (a)

M11 =

M11 TN−1 (a) − TN−2 (a)

cosˇ1 cosˇ2 cosˇ3 −

=

M12 = −i

+

m11

m12

m21

m22

(2)

p2 sinˇ1 sinˇ2 cosˇ3 p1

p3 cosˇ1 sinˇ2 sinˇ3 p3 sinˇ1 cosˇ2 sinˇ3 − − p2 p1

(3)

cosˇ1 sinˇ2 cosˇ3 sinˇ1 cosˇ2 cosˇ3 + p1 p2

cosˇ1 cosˇ2 sinˇ3 p2 sinˇ1 sinˇ2 sinˇ3 − p3 p1 p2

(4)

M21 = −i p1 sinˇ1 cosˇ2 cosˇ3 + p2 cosˇ1 sinˇ2 cosˇ3 p1 p3 sinˇ1 sinˇ2 sinˇ3 +p3 cosˇ1 cosˇ2 sinˇ3 − p2

M 22 = −

cosˇ1 cosˇ2 cosˇ3 −

,

(5)

p1 sinˇ1 sinˇ2 cosˇ3 p2

p2 cosˇ1 sinˇ2 sinˇ3 p1 sinˇ1 cosˇ2 sinˇ3 − p3 p3

Figure 1 shows a schematic diagram of the proposed photonic crystal. It consists of three layers having the indices n1 , n2 and n3 with thicknesses d1 , d2 and d3 , respectively. The period of the lattice is given by d = d1 +d2 +d3 . Layer 2 is considered LHM of negative parameters (ε2 , 2 ). The index of refraction n2 can be calculated as √ n2 = − ε2 2 . The characteristic matrix of a cell consisting of three layers is given by

p1 =

2

1−

1−

(6)

TN are well-known functions called Chebyshev polynomials of the second kind

2. Theory

i=1

, cos2 =

n21

and cos3 =

12

ε1 1 cos1 ,

M11

M12

M21

M22

(1)

1 − a2

12

,

(7)

where a=

1 [M11 + M22 ]. 2

(8)

Using the matrix elements mij , the transmission coefﬁcient of the stack of layers can be written as t=

2p0 . (m11 + m12 p0 ) p0 + (m21 + m22 p0 )

(9)

where

2 =

ε2 2 cos2

⎦=

cosˇi

2n1 d1 cos 1 , 0

p2 =

⎤

TN (a) =

sin (N + 1) cos−1 a

2n2 d2 cos 2 , 0

and p3 =

3 =

2(n3 )d3 cos 3 , 0

ε3 3 cos3 .

and o is

the free space wavelength. 1 , 2 and 3 are the angles which the ray makes with the normal to the interfaces in layers 1, 2 and 3, respectively. They are

po = n0 cos 0 = cos0 .

(10)

with n0 = 1. The transmittance is then given by T = |t|2 .

(11)

238

S.A. Taya / Opto-Electronics Review 26 (2018) 236–241

Fig. 2. Transmittance vs. wavelength for the ternary photonic crystal with different values of n3 for N = 6, n1 = 1.54, ε2 = −5.5 + 0.01i, 2 = − 5.0 + 0.01i, n2 = −

(−5.5 + 0.01i)(−5.0 + 0.01i), d1 = 100 nm, d2 = 30 nm, and d3 = 100 nm.

3. Results and discussion A ternary photonic crystal was assumed with the structure dielectric / LHM / air. The following parameters are assumed N = 6, n 1 = 1.54, ε2 = −5.5 + 0.01i [28], 2 = − 5.0 + 0.01i [28], n2 = − (−5.5 + 0.01i)(−5.0 + 0.01i), d1 = 100 nm, d2 = 30 nm, and d3 = 100 nm. We ﬁrst assume normal incidence of o = 0◦ . The transmission spectrum of the one-dimensional ternary photonic crystal is shown in Fig. 2 for n3 = 0.02, 0.04, and 0.06. The wavelength was varied from 1350 nm to 1650 nm in steps of 0.1 nm. It was observed that the transmission spectrum of the ternary photonic crystal shows narrow transmission peaks. The peak shifts toward larger wavelengths for any increase in the refractive index of the analyte is clear. This shift in the transmission spectrum is the key in the sensing process. Solid, dashed, dotted and dash dotted curves correspond to n3 = 1.00, 1.02, 1.04 and 1.06. The solid curve transmission peak has a central wavelength at 1459.9 nm for n3 = 0.00. The dashed curve transmission peak has a central wavelength at 1461 nm whereas the dotted curve is centered at 1462.2 for n3

= 0.02 and 0.04, respectively. The dashed dotted curve has its center at a wavelength of 1463.4 for n3 = 0.06. The sensitivity of the proposed sensor can be evaluated as /n which is given by 58.3 nm. This is a high shift and can be detected easily with existing optoelectronic devices. We now try to optimize ε2 and d2 of the LHM to ﬁnd out the values corresponding to the maximum shift in the transmission peak. Figure 3 shows the transmission spectrum of the one-dimensional ternary photonic crystal for ε2 = −6.0 + 0.01i, −5.5 + 0.01i, −5.0 + 0.01i and −4.5 + 0.01i. The transmission spectrum of the ternary photonic crystal shows transmission peak shifts for any increase in the refractive index of the analyte. Solid, dashed, dotted and dash dotted curves correspond to n3 = 1.00, 1.02, 1.04 and 1.06. For ε2 = −6.0 + 0.01i (upper left panel), the sensitivity of the photonic crystal sensor is found to be /n = 56.67 nm. When ε2 is decreased to ε2 = −5.5 + 0.01i (upper right panel), the sensitivity is found to be /n = 58.3 nm. If ε2 is decreased again to ε2 = −5.0 + 0.01i (lower left panel), the sensitivity is /n = 61.67 nm. Finally if ε2 is decreased to become ε2 = −4.5 + 0.01i, we ﬁnd that /n = 105 nm. As can be seen from Fig. 3, the wavelength shift can be considerably enhanced with the decrease of the absolute value of the real part of the LHM permittivity. The transmission spectrum of the one-dimensional ternary photonic crystal is plotted in Fig. 4 for d2 = 24 nm, 26 nm, 28 nm and 30 nm. The transmission peaks shift for any increase in the refractive index of the analyte can be seen clearly in the ﬁgure. For d2 = 24 nm, the solid curve transmission peak has a central wavelength at 1534.6 nm for n3 = 0.00 whereas the dashed curve transmission peak has a central wavelength at 1536.6 nm for n3 = 0.02. The dotted curve is centered at 1538.7 for n3 = 0.04 and the dashed dotted curve has its center at a wavelength of 1540.9 for n3 = 0.06. As seen, the transmission peak exhibits a wavelength shift of 6.3 nm for n3 = 0.06 revealing a sensitivity of /n = 105 nm. On the other hand it shows a sensitivity of /n = 101 nm, 61.67 nm, and 58.33 for d2 = 26 nm, 28 nm and 30 nm, respectively. As observed from Fig. 4, the wavelength shift can be signiﬁcantly improved with the decrease of the LHM thickness. If we move to the oblique incidence and examine the wavelength shift with the angle of incidence as illustrated in Fig. 5. As

Fig. 3. Transmittance vs. wavelength for the ternary photonic crystal with different values of n3 for different values of ε2 , N = 6, n1 = 1.54, 2 = − 5.0 + 0.01i, n2 = −

ε2 (−5.0 + 0.01i), d1 = 100 nm, d2 = 30 nm, and d3 = 100 nm.

S.A. Taya / Opto-Electronics Review 26 (2018) 236–241

239

Fig. 4. Transmittance vs. wavelength for the ternary photonic crystal with different values of n3 for different values of d2 , N = 6, n1 = 1.54, ε2 = −5.5 + 0.01i, 2 = − 5.0 + 0.01i, n2 = −

(−5.5 + 0.01i)(−5.0 + 0.01i), d1 = 100 nm, and d3 = 100 nm.

Fig. 5. Transmittance vs. wavelength for the ternary photonic crystal with different values of n3 for different values of the incidence angle, N = 6, n1 = 1.54, ε2 = −5.5 + 0.01i,

2 = − 5.0 + 0.01i, n2 = −

(−5.5 + 0.01i)(−5.0 + 0.01i), d1 = 100 nm, and d3 = 100 nm.

can be seen from the ﬁgure, the incidence angle has no effect of the wavelength shift. For o = 0◦ , 30◦ , 45◦ and 60◦ , the wavelength shift reaches 3.5 nm for all angles of incidence for n3 = 1.06 compared to n3 = 1.00 and the sensitivity is estimated as /n = 58.33 nm. It is worth comparing the results of the current work with the state of the art sensitivity. In a recent work [5], a ternary photonic crystal was proposed as a refractometric sensor for detection small changes in the index of refraction of an analyte. The obtained sensitivity in their work was /n = 350 nm whereas we could achieve a sensitivity of about /n = 105 nm for some conﬁguration of the proposed photonic crystal. However, the obtained sensitivity can be adjusted and considerably increased by choosing the appropriate parameters of the LHM.

4. Conclusions One-dimensional ternary photonic crystal with left-handed material layer is examined for refractometric applications. One of the layers is assumed to be air and treated as an analyte. The transmission spectrum from the one-dimensional ternary photonic crystal is studied in details and the wavelength shift due to the change in the index of an analyte is investigated with different parameters of the structure. It was observed that the transmission peak shows a shift of 0.583 nm for each refractive index change of 0.01. This shift is high enough to be detected easily with existing optoelectronic devices. The sensitivity of the proposed sensor was evaluated as /n and found 58.3 nm. We studied the

240

S.A. Taya / Opto-Electronics Review 26 (2018) 236–241

sensitivity with the permittivity of the LHM and found that for ε2 = −6.0 + 0.01i, ε2 = −5.5 + 0.01i, ε2 = −5.0 + 0.01i and ε2 = −4.5 + 0.01i the proposed photonic crystal has the sensitivities /n = 56.67 nm, 58.3 nm, 61.67 nm and 105 nm, respectively. Moreover, we investigated the wavelength shift with the LHM thickness and observed that for d2 = 24 nm, 26 nm, 28 nm and 30 nm the structure exhibited sensitivities of /n = 105 nm, 101 nm, 61.67 nm and 58.33, respectively. The wavelength shift can be signiﬁcantly improved with the decrease of the LHM thickness and the LHM permittivity. We also found that the incidence angle has no effect of the wavelength shift.

where

Appendix A.

Now differentiating Eq. (A.4) with respect to z and substituting from Eq. (A.5), we get

Let the plane of incidence be y–z plane, then for TE mode, Ey = Ez = 0. The solution of the wave equation can be written as [29]

d2 U 2 + k0 n2 − b2 U = 0. 2 dz

Ex = U(z)e

i(k0 by−ωt)

(A.1)

i(k0 by−ωt)

(A.2)

H y = V (z)e

Hz = W (z)ei(k0 by−ωt)

(A.3)

where k0 is the wavenumber in the vacuum, is the wave frequency and b = n sin, where denotes the angle which the ray makes with the normal and n is the index of refraction. After substitutions in Maxwell’s equation, U, V and W are related to each other by the following equations U` = ik0 V

(A.4)

V` = ik0 (ε −

b2 )U

Q =

(A.6)

, Q0 =

V (z)

U0

,N=

V0

F(z)

f (z)

G(z) g(z)

,

(A.19)

then Q0 = MQ

(A.20)

where M= [

−f (z)

g(z)

−G(z) F(z)

(A.21)

].

(A.22)

Differentiating Eq. (A.5) with respect to z and substituting from Eq. (A.4), we get

d2 V 2 + k0 n2 − b2 V = 0. 2 dz

(A.23)

Substituting for b = n sin d2 U dz 2

2

+ (k0 n2 cos2 )U = 0.

(A.24)

d2 V 2 + +(k0 n2 cos2 )V = 0. dz 2

(A.25)

The solution of the above equations is given by

(A.5)

bU + W = 0

U(z)

U(z) = Acos(k0 nzcos) + Bsin(k0 nzcos) 1 i

(A.26)

ε cos Bcos ko nzcos − Asin(k0 nzcos) .

U, V can be expressed as combinations of two particular solutions as

V (z) =

U`1 = ik0 V1

Applying the boundary condition in Eq. (A.15) and making use of Eq. (A.14), we get

(A.7)

U`2 = ik0 V2 , V`1

= ik0 (ε −

V`2

= ik0

(A.8)

b2

U1 = f (z) = (A.9)

)U1

b2 ε−

U2 .

(A.10)

− V1` U2

V1 U`2

− U`1 V2

=0 =0

d (U1 V2 − U2 V1 ) = 0 dZ

(A.11) (A.12)

U1 = f (z) , U 2 = F (z) , V1 = g (z) , V2 = G(z) such that f (0) = G (0) = 0 and F(0) = g(0) = 1.

(A.15)

The solutions with U(0) = U0 , V (0) = V0 may be expressed in the form U = FU0 + fV0 ,

(A.16)

V = GU0 + gV0 .

(A.17)

or in matrix notation Q = NQ0

(A.18)

(A.28)

(A.29)

V1 = g(z) = cos(k0 nzcos)

(A.30)

U0

⎛ =⎝

(A.13)

(A.14)

sin(k0 nzcos) ε

U2 = F (z) = cos k0 nzcos ,

V0

For our purpose, the most convenient choice of the particular solution is

V 2 = G(z) = i

The relations (7–10) follow that U1 V2`

i cos

(A.27)

ε sin(k0 nzcos)

cos(k0 nzcos) −ipsin(k0 nzcos)

(A.31)

⎞

i − sin(k0 nzcos) p ⎠ U . (A.32) V cos(ko nzcos)

References [1] S. Sandhu, S. Fan, M. Yanik, M. Povinelli, Advances in theory of photonic crystal, J. Light Wave Technol. 24 (2006) 4493–4501. [2] I. Kriegel, F. Scotognella, Disordered one-dimensional photonic structures composed by more than two materials with the same optical thickness, Opt. Commun. 338 (2015) 523–527. [3] Z. Zare, A. Gharaati, Investigation of band gap width in ternary 1D photonic crystal with left-handed laye, Acta Phys. Pol. A 125 (2014) 36–38. [4] C.J. Wu, Y.H. Chung, T.J. Yang, B.J. Syu, Band gap extension in a one-dimensional ternary metal-dielectric photonic crystal, Prog. Electromagn. Res. 102 (2010) 81–93. [5] A. Banerjee, Enhanced refractometric optical sensing by using one-dimensional ternary photonic crystals, Prog. Electromagn. Res., PIER 89 (2009) 11–22. [6] S.K. Awasthi, U. Malaviya, S.P. Ojha, Enhancement of omnidirectional total-reﬂection wavelength range by using one dimensional ternary photonic band gap material, J. Opt. Soc. Am. B 23 (2006) 2566–2571. [7] F. Xue, S. Liu, H. Zhang, X. Kong, Y. Wen, Wang L, S. Qian, The theoretical analysis of omnidirectional photonic band gaps in the one-dimensional

S.A. Taya / Opto-Electronics Review 26 (2018) 236–241

[8]

[9]

[10]

[11] [12] [13]

[14] [15] [16] [17] [18]

ternary plasma photonic crystals based on Pell quasi-periodic structure, Opt. Quant. Electron. 49 (2017) 19. S. Sharma, R. Kumar, K. Singh, A. Kumar, V. Kumar, Omnidirectional reﬂector using linearly graded refractive index proﬁle of 1D binary and ternary photonic crystal, Optik 126 (2015) 1146–1149. S.K. Awasthi, S.P. Ojha, Design of a tunable optical ﬁlter by using one-dimensional ternary photonic band gap material, Prog. Electromagn. Res. M 4 (2008) 117–132. A. Banerjee, Enhanced temperature sensing by using one-dimensional ternary photonic band gap structures, Prog. Electromagn. Res. Lett. 11 (2009) 129–137. V.G. Veselago, The electrodynamics of substances with simultaneously negative values of and , Sov. Phy. Usp. 10 (1968) 509–514. J.B. Pendry, A.J. Holden, W.J. Stewart, I. Youngs, Extremely low frequency plasmons in mettalic mesostructures, Phys. Rev. Lett. 76 (1996) 4773–4776. J.B. Pendry, A.J. Holden, D.J. Robbins, W.J. Stewart, Magnetism from conductors and enhanced nonlinear phenomena, IEEE. Trans. Microw. Theory Tech. 47 (1999) 2075–2090. R.A. Shelby, D.R. Smith, S. Schultz, Experimental veriﬁcation of a negative index of refraction, Science 292 (2001) 77–79. S.A. Taya, Dispersion properties of lossy, dispersive, and anisotropic left-handed material slab waveguide, Optik 126 (2015) 1319–1323. S.A. Taya, Theoretical investigation of slab waveguide sensor using anisotropic metamaterials, Opt. Appl. 45 (2015) 405–417. K. Tiefenthaler, W. Lukosz, Sensitivity of grating couplers as integrated-optical chemical sensors, J. Opt. Soc. Am. B 6 (1989) 209–220. R. Horvath, G. Fricsovszky, E. Pap, Application of the optical waveguide light mode spectroscopy to monitor lipid bilayer phase transition, Biosens. Bioelectron. 18 (2003) 415–428.

241

[19] B. Kuswandi, Simple optical ﬁber biosensor based on immobilized enzyme for monitoring of trace having metal ions, Anal. Bioanal. Chem. 376 (2003) 1104–1110. [20] E. Udd, An overview of ﬁber optic sensors, Rev. Sci. Instrum. 66 (1995) 4015–4030. [21] F.C. Chien, S.J. Chen, A sensitivity comparison of optical biosensors based on four different surface plasmon resonance modes, Biosens. Bioelectron. 20 (2004) 633–642. [22] J. Homola, S.S. Yee, G. Gauglitz, Surface plasmon resonance sensors: review, Sens. Actuators B 54 (1999) 3–15. [23] N. Skivesen, R. Horvath, H. Pedersen, Optimization of metal-clad waveguide sensors, Sens. Actuators B 106 (2005) 668–676. [24] N. Skivesen, R. Horvath, H. Pedersen, Peak-type and dip-type metal-clad waveguide sensing, Opt. Lett. 30 (2005) 1659–1661. [25] N. Skivensen, R. Horvath, S. Thinggaaed, N.B. Larsen, H.C. Pedersen, Deep-probe metal-clad waveguide biosensors, Biosens. Bioelectron. 22 (2007) 1282–1288. [26] S.A. Taya, Slab waveguide with air core layer and anisotropic left-handed material claddings as a sensor, Opto-Electron. Rev. 22 (2014) 252–257. [27] S.A. Taya, P-polarized surface waves in a slab waveguide with left-handed material for sensing applications, J. Magn. Magn. Mater. 377 (2015) 281–285. [28] G. Wu, Song Liu, S. Zhong, Numerical analysis of propagation characteristics of electromagnetic wave in lossy left-handed material media, Optik 125 (2014) 4233–4237. [29] M. Born, E. Wolf, Principles of Optics, Cambridge University Press, United Kingdom, 2003.

Copyright © 2022 COEK.INFO. All rights reserved.